adsorption of co2 on polyethyleneimine file.scirp.org/pdf/ajac_ solid sorbent based on...
Post on 06-Apr-2018
Embed Size (px)
American Journal of Analytical Chemistry, 2015, 6, 274-284 Published Online March 2015 in SciRes. http://www.scirp.org/journal/ajac http://dx.doi.org/10.4236/ajac.2015.64026
How to cite this paper: Khader, M.M., Al-Marri, M.J., Ali, S., Qi, G. and Giannelis, E.P. (2015) Adsorption of CO2 on Polye-thyleneimine 10kMesoporous silica Sorbent: XPS and TGA Studies. American Journal of Analytical Chemistry, 6, 274-284. http://dx.doi.org/10.4236/ajac.2015.64026
Adsorption of CO2 on Polyethyleneimine 10kMesoporous silica Sorbent: XPS and TGA Studies M. M. Khader1*, M. J. Al-Marri1, Sardar Ali1, G. Qi2, E. P. Giannelis2 1Gas Processing Center, College of Engineering, Qatar University, Doha, Qatar 2Department of Materials Science and Engineering, Cornell University, Ithaca, NY, USA Email: *email@example.com Received 27 January 2015; accepted 2 March 2015; published 6 March 2015
Copyright 2015 by authors and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY). http://creativecommons.org/licenses/by/4.0/
Abstract A CO2 solid sorbent based on polyethyleneimine 10k (PEI-10k) impregnated into mesoporous sil-ica (MPS) foam was synthesized and utilized to capture CO2 at temperatures ranged from 65C to 95C. The calculated nitrogen and carbon contents in the bulk of the PEI-10k/MPS sorbent were similar to the XPS results measured on the surface of the foam, suggesting that the PEI was homo- geneously distributed throughout the MPS support. After CO2 adsorptionthe N 1s peak was bro- adened and could be resolved into two components: a high binding energy component (~401 eV) and a lower binding energy one (396 eV), respectively. The former nitrogen states are consistent with a protonated amine, presumably, due to carbamate formation. The lower binding energy component (~396 eV) could possibly be due to strongly chemisorbed CO2. The maximum sorption capacity was about 4 mmole CO2/g sorbent at 85C and 1 bar. This capacity was doubled by raising the CO2 pressure to 24.95 bars. The adsorption results can be described by a Langmuir adsorption isotherm.
Keywords XPS, Adsorption Isotherm of CO2, Polyethyleneimine 10k, Mesoporous silica
1. Introduction Carbon dioxide is one of the major greenhouse gases (GHGs). Starting early in 19th century, extensive anthro-pogenic CO2 emissions due to fossil fuel utilization have led to carbon dioxide accumulation in the atmosphere.
M. M. Khader et al.
According to the Intergovernmental Panel on Climate Change (IPCC) the increase in greenhouse gases has trig-gered serious climate changes demonstrated more obviously as an increase in earth temperature. In this context, the development of highly efficient CO2 sorbents for trapping large amounts of CO2 from concentrated sources such as natural gas processing and power plants emission emerges as a pressing issue. Among several available processes for carbon dioxide capture, CO2 capture with amines is a well-established technology -. Still, al-ternative processes such as effective and less expensive solid CO2 sorbents based on amine immobilization on porous supports are extensively investigated with the goal to develop recyclable solid sorbents to achieve com-petitive and less energy intensive acid-gas removal alternatives -. Unlike liquid sorbents, solid sorbents yield less waste during cycling. Additionally, the spent solid sorbents can be disposed more easily and in an en-vironmentally friendly way. There still remain several challenges before amine immobilized CO2 sorbents be-come industrially practical. High-surface-area silica such as MCM-41 , MCM-22, MCM-36 and ITQ-2  and many others  have been widely used as supports for immobilizing various types of amines for CO2 cap-ture. In particular, amine functionalized solid sorbents are appealing - because the high capture capacity of the amine molecules is retained  . Various other adsorbents such as zeolites  , activated car-bons -, activated aluminas -, and membranes  have also been investigated. Zeolite based sorbents showed high adsorption capacity at lower temperatures, but their capacity declines above room temper-ature  . In addition, since these sorbents also absorb moisture and other gases, their CO2 separation se-lectivity is low, resulting in large separation systems with high operational cost in practical applications.
Grafting of amines on porous solids is one way to enhance the adsorption capacity of sorbents  . Sol-id-supported amines possess significant advantages such as low energy cost for sorbent regeneration, high selec-tivity and reversibility towards CO2 and ease of disposal. In addition, solid amine sorbents have been proved to be tolerant towards moisture and, thus, more effective for capturing humidified CO2 compared with zeolites and activated carbons -. Among various solids which could be functionalized with amines for CO2 sorption, Mesoporous silica have been attracted much attention -. This category of porous materials possesses several desirable properties such as large surface area, tuneable pore structure, and high thermal stability. These properties make Mesoporous silica a promising support for amine immobilization. To date a series of amine supported Mesoporous silica have been prepared and investigated -. In general, Mesoporous silica foams with large pore size and pore volume are better supports compared to other mesoporous siliceous mate-rials. Amine functionalized supports such as MCM-41 , MCM-22 and ITQ-2  showed lower CO2 capaci-ties. On the other hand, these amine based sorbents showed better selectivity for CO2 adsorption over N2 or CH4.  .
The objective of this work was to investigate the CO2 sorption mechanism on amine functionalized Meso-porous silica and maximize the sorption capacity. A properly designed PEI/MPS sorbent was synthesized for use intheCO2 sorption studies. XPS was employed to follow changes in the surface chemical bonding while CO2 was interacted with the solid sorbent. Lastly, high CO2 pressure adsorption experiments were conducted in an effort to enhance the sorption capacity of the hybrid sorbent.
2. Experimental 2.1. Chemicals Triblock co-polymer poly (ethylene oxide)-b-(propylene oxide)-b-poly(ethylene oxide) surfactant P123 (EO20PO70- EO20, Mv = 5800), sodium silicate, acetic acid, ammonium fluoride, polyethylenimine, PEI10K, Mn 10,000), Span 80 surfactant and ethanol (v/v = 90%) were all purchased from Aldrich and used without further purifica-tion. Deionized water was used in all experiments.
2.2. Preparation of Foam Support The Mesoporous silica (MPS) support was prepared as reported previously  . Briefly 3.0 g of P123 was dissolved in a solution of acetic acid (3.0 g), water (52 g), and ammonium fluoride (0.3 g) at 40C. A solution of sodium silicate (2.35 g) in water (40 g) was heated to 40C and poured into the surfactant solution under vigor-ous stirring. The mixture was kept under static conditions at 40C for 24 h and aged at 70C for another 24 h. The product was collected by filtration, followed by copiously washing with DI water. The surfactant P123 was removed by calcination at 560C for 6 h.
M. M. Khader et al.
2.3. Sorbent Preparation PEI-10K (10,000 g/mol) was impregnated into the Mesoporous silica. In a typical batch, a certain amount of PEI was added into 10 mL of dry ethanol. After dissolution, 1 g of Mesoporous silica was added under stirring fol-lowed by statically keeping the mixture at room temperature for 12 h. The resultant slurry was dried at 100C for 16 h. The obtained sample was denoted as PEI10K-MPS.
2.4. CO2 Sorption/Desorption Performance The CO2 sorption-desorption of the PEI/MPS sorbents were monitored using a Pyris 6 TGA Perkin Elmer ther-mal gravimetric analyzer (TGA) by following the weight increases/decreases during the sorption and desorption process in pure CO2. About 10 mg of the sorbent was put into the TGA measuring pan, the temperature was in-creased from room temperature to 110C at a heating rate of 5C/min and equilibrated at 110C for 30 min under pure N2 (99.99%) at a flow rate of 20 ml/min to remove any moisture or remaining solvent from the sorbents. The temperature was then allowed to drop to the desired sorption temperature and the gas was switched from N2 to pure CO2 (99.9%), held for 90 min for CO2 sorption, and then switched back to N2 for 30 min for CO2 de-sorption while the temperature was kept fixed. The CO2 sorption capacity (mmol CO2/g sorbent) was calculated from the weight change of the sample measured by TGA during the sorption/ desorption processes. Note that the sorption capacity measured by TGA in this study is an equilibrium sorption capacity, as CO2 was allowed to flow till the weight of the sample reached its maximum value. The high pressure CO2 adsorption capacity was determined using a Rubotherm Magnetic Suspension Balance (MSB). In a typical high pressure CO2 adsorp-tion-desorption isotherm measurement, approximately 50 mg of PEI-10k/MPS was placed on an alumina cruci-ble. The system was taken under vacuum for 3 h at 85C. CO2 adsorption isotherms were measured at 85C by raising the pressure from ambient to 30 atm.
2.5. Characterization Techniques Surface areas were calculated by the simplified Broekhoff-de Boer method from N2 sorption experiments. The total pore volume was estimated from the amount of N2adsorbed at a relative pressure of 0.99. The pore size and t